#------------------------------------------------------------------------------
#$Date: 2023-09-05 22:18:14 +0300 (Tue, 05 Sep 2023) $
#$Revision: 286059 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/94/1569432.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1569432
loop_
_publ_author_name
'Murali, Meenu'
'Bijani, Christian'
'Daran, Jean-Claude'
'Manoury, Eric'
'Poli, Rinaldo'
_publ_section_title
;
 Acetate exchange mechanism on a Zr₁₂ oxo hydroxo cluster:
 relevance for reshaping Zr-carboxylate coordination adaptable networks.
;
_journal_issue                   30
_journal_name_full               'Chemical science'
_journal_page_first              8152
_journal_page_last               8163
_journal_paper_doi               10.1039/d3sc02204h
_journal_volume                  14
_journal_year                    2023
_chemical_formula_sum            'C28 H50 O37 Zr6'
_chemical_formula_weight         1526.00
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2023-04-02 deposited with the CCDC.	2023-07-04 downloaded from the CCDC.
;
_cell_angle_alpha                100.5670(10)
_cell_angle_beta                 109.8910(10)
_cell_angle_gamma                104.9940(10)
_cell_formula_units_Z            2
_cell_length_a                   12.50240(10)
_cell_length_b                   16.6275(2)
_cell_length_c                   17.2067(2)
_cell_measurement_reflns_used    35976
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      76.2500
_cell_measurement_theta_min      2.8550
_cell_volume                     3100.64(7)
_computing_cell_refinement       CrysAlisPro
_computing_data_collection
'CrysAlisPro  (Rigaku Oxford Diffraction, 2018)'
_computing_data_reduction        CrysAlisPro
_computing_molecular_graphics
'ORTEPIII (Burnett & Johnson, 1996); ORTEP-3 for Windows (Farrugia, 1997)'
_computing_publication_material  SHELXL-2015
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXt (Sheldrick, 2015)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      100(2)
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 10.0000
_diffrn_detector_type            HyPix
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.947
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB Synergy, Dualflex, HyPix'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0371
_diffrn_reflns_av_unetI/netI     0.0248
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.947
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            57874
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.947
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         77.005
_diffrn_reflns_theta_min         2.862
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_type              'PhotonJet (Cu) X-ray Source'
_exptl_absorpt_coefficient_mu    8.746
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.68732
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.41.120a (Rigaku Oxford Diffraction, 2021)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.634
_exptl_crystal_description       box
_exptl_crystal_F_000             1508
_exptl_crystal_size_max          0.100
_exptl_crystal_size_mid          0.050
_exptl_crystal_size_min          0.050
_refine_diff_density_max         1.499
_refine_diff_density_min         -1.339
_refine_diff_density_rms         0.125
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.081
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     662
_refine_ls_number_reflns         12418
_refine_ls_number_restraints     7
_refine_ls_restrained_S_all      1.082
_refine_ls_R_factor_all          0.0395
_refine_ls_R_factor_gt           0.0370
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0728P)²+2.7927P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1077
_refine_ls_wR_factor_ref         0.1097
_reflns_number_gt                11286
_reflns_number_total             12418
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d3sc02204h2.cif
_cod_data_source_block           '[Zr6O4(OH)4(O2CMe)12]2'
_cod_depositor_comments          'Adding full bibliography for 1569432.cif.'
_cod_original_cell_volume        3100.64(6)
_cod_database_code               1569432
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.475
_shelx_estimated_absorpt_t_max   0.669
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Zr1 Zr 0.36042(2) 0.37732(2) 0.05259(2) 0.01910(7) Uani 1 1 d . . . . .
Zr2 Zr 0.65045(2) 0.35086(2) 0.10443(2) 0.01889(7) Uani 1 1 d . . . . .
Zr3 Zr 0.66284(2) 0.34313(2) 0.30871(2) 0.02032(8) Uani 1 1 d . . . . .
Zr4 Zr 0.38190(2) 0.37241(2) 0.25704(2) 0.02127(8) Uani 1 1 d . . . . .
Zr5 Zr 0.62175(2) 0.52155(2) 0.24049(2) 0.01997(8) Uani 1 1 d . . . . .
Zr6 Zr 0.40984(2) 0.20113(2) 0.12000(2) 0.02003(8) Uani 1 1 d . . . . .
O11 O 0.21469(19) 0.26095(14) -0.04573(14) 0.0227(4) Uani 1 1 d . . . . .
O12 O 0.19320(19) 0.39204(14) 0.06001(15) 0.0240(4) Uani 1 1 d . . . . .
O14 O 0.35777(19) 0.50409(14) 0.03032(14) 0.0216(4) Uani 1 1 d . . . . .
O15 O 0.37890(19) 0.37790(14) -0.07013(14) 0.0221(4) Uani 1 1 d . . . . .
O21 O 0.81826(18) 0.32764(14) 0.17072(15) 0.0229(4) Uani 1 1 d . . . . .
O22 O 0.6175(2) 0.22071(14) 0.02129(14) 0.0236(4) Uani 1 1 d . . . . .
O25 O 0.80300(19) 0.47021(14) 0.12962(15) 0.0237(4) Uani 1 1 d . . . . .
O31 O 0.8120(2) 0.46112(15) 0.40736(14) 0.0256(5) Uani 1 1 d . . . . .
O32 O 0.83197(19) 0.32891(15) 0.30453(15) 0.0253(5) Uani 1 1 d . . . . .
O33 O 0.6574(3) 0.32696(16) 0.43638(17) 0.0348(6) Uani 1 1 d . . . . .
O34 O 0.6659(2) 0.21983(16) 0.34790(16) 0.0300(5) Uani 1 1 d . . . . .
O41 O 0.3991(2) 0.50457(15) 0.33138(15) 0.0279(5) Uani 1 1 d . . . . .
O42 O 0.2082(2) 0.39405(15) 0.19386(15) 0.0258(5) Uani 1 1 d . . . . .
O43 O 0.3828(2) 0.35538(16) 0.38446(16) 0.0313(5) Uani 1 1 d . . . . .
O44 O 0.2405(2) 0.25854(16) 0.26646(16) 0.0299(5) Uani 1 1 d . . . . .
O51 O 0.7866(2) 0.58054(14) 0.21618(15) 0.0251(4) Uani 1 1 d . . . . .
O52 O 0.4013(2) 0.36816(14) -0.19306(14) 0.0240(4) Uani 1 1 d . . . . .
O53 O 0.7782(2) 0.57494(15) 0.36399(15) 0.0264(5) Uani 1 1 d . . . . .
O54 O 0.5584(2) 0.59777(15) 0.32384(15) 0.0259(5) Uani 1 1 d . . . . .
O55 O 0.3601(2) 0.63568(14) 0.02207(14) 0.0236(4) Uani 1 1 d . . . . .
O61 O 0.24617(19) 0.14517(15) -0.00580(15) 0.0248(4) Uani 1 1 d . . . . .
O62 O 0.4596(2) 0.12450(14) 0.02815(15) 0.0239(4) Uani 1 1 d . . . . .
O63 O 0.4434(2) 0.09566(15) 0.18240(16) 0.0288(5) Uani 1 1 d . . . . .
O64 O 0.2692(2) 0.11364(15) 0.15182(17) 0.0297(5) Uani 1 1 d . . . . .
O135 O 0.56277(18) 0.45662(13) 0.09665(14) 0.0197(4) Uani 1 1 d D . . . .
H135 H 0.585109 0.505260 0.067912 0.030 Uiso 1 1 d DR U . . .
O136 O 0.46384(18) 0.29813(13) 0.06770(14) 0.0201(4) Uani 1 1 d . . . . .
O145 O 0.43951(19) 0.44328(14) 0.18352(14) 0.0209(4) Uani 1 1 d . . . . .
O146 O 0.29671(19) 0.28321(14) 0.12417(14) 0.0208(4) Uani 1 1 d D . . . .
H146 H 0.205086 0.248660 0.099075 0.031 Uiso 1 1 d DR U . . .
O235 O 0.67406(18) 0.41493(13) 0.22591(13) 0.0199(4) Uani 1 1 d . . . . .
O236 O 0.60870(19) 0.24934(14) 0.18014(14) 0.0210(4) Uani 1 1 d D . . . .
H236 H 0.663513 0.220416 0.191907 0.031 Uiso 1 1 d DR U . . .
O346 O 0.47361(19) 0.28477(14) 0.24686(14) 0.0219(4) Uani 1 1 d . . . . .
O356 O 0.57714(19) 0.44031(14) 0.33306(14) 0.0223(4) Uani 1 1 d D . . . .
H356 H 0.617204 0.466639 0.394087 0.033 Uiso 1 1 d DR U . . .
C35 C 0.6604(3) 0.2507(2) 0.4197(2) 0.0319(7) Uani 1 1 d . . . . .
C36 C 0.6572(6) 0.1972(3) 0.4797(3) 0.0583(13) Uani 1 1 d . . . . .
H36A H 0.576492 0.179693 0.480298 0.087 Uiso 1 1 calc R U . . .
H36B H 0.717989 0.231457 0.538173 0.087 Uiso 1 1 calc R U . . .
H36C H 0.675158 0.144985 0.460143 0.087 Uiso 1 1 calc R U . . .
C45 C 0.2907(3) 0.2849(2) 0.3477(2) 0.0286(7) Uani 1 1 d . . . . .
C46 C 0.2447(4) 0.2349(3) 0.4007(3) 0.0438(9) Uani 1 1 d . . . . .
H46A H 0.161408 0.194969 0.365073 0.066 Uiso 1 1 calc R U . . .
H46B H 0.246164 0.275628 0.450404 0.066 Uiso 1 1 calc R U . . .
H46C H 0.296554 0.201354 0.421433 0.066 Uiso 1 1 calc R U . . .
C65 C 0.3432(3) 0.0783(2) 0.1890(2) 0.0271(7) Uani 1 1 d . . . . .
C66 C 0.3128(4) 0.0205(3) 0.2410(3) 0.0508(11) Uani 1 1 d . . . . .
H66A H 0.342108 -0.028190 0.232162 0.076 Uiso 1 1 calc R U . . .
H66B H 0.224617 -0.002212 0.222572 0.076 Uiso 1 1 calc R U . . .
H66C H 0.351557 0.054003 0.302564 0.076 Uiso 1 1 calc R U . . .
C141 C 0.1529(3) 0.3965(2) 0.1183(2) 0.0271(7) Uani 1 1 d . . . . .
C142 C 0.0297(3) 0.4049(3) 0.0950(3) 0.0391(9) Uani 1 1 d . . . . .
H14A H -0.032111 0.346867 0.075952 0.059 Uiso 1 1 calc R U . . .
H14B H 0.013258 0.431780 0.048179 0.059 Uiso 1 1 calc R U . . .
H14C H 0.027768 0.441368 0.145832 0.059 Uiso 1 1 calc R U . . .
C143 C 0.3455(3) 0.5756(2) 0.0576(2) 0.0235(6) Uani 1 1 d . . . . .
C144 C 0.3147(3) 0.5934(2) 0.1340(2) 0.0274(7) Uani 1 1 d . . . . .
H14D H 0.227429 0.582271 0.114155 0.041 Uiso 1 1 calc R U . . .
H14E H 0.359632 0.654483 0.169137 0.041 Uiso 1 1 calc R U . . .
H14F H 0.336882 0.555197 0.168970 0.041 Uiso 1 1 calc R U . . .
C151 C 0.3835(3) 0.33440(19) -0.1363(2) 0.0220(6) Uani 1 1 d . . . . .
C152 C 0.3687(3) 0.2395(2) -0.1510(2) 0.0271(7) Uani 1 1 d . . . . .
H15A H 0.389215 0.226715 -0.095431 0.041 Uiso 1 1 calc R U . . .
H15B H 0.422896 0.226282 -0.177259 0.041 Uiso 1 1 calc R U . . .
H15C H 0.284527 0.203684 -0.189755 0.041 Uiso 1 1 calc R U . . .
C161 C 0.1837(3) 0.1795(2) -0.0546(2) 0.0247(6) Uani 1 1 d . . . . .
C162 C 0.0658(3) 0.1227(2) -0.1281(2) 0.0307(7) Uani 1 1 d . . . . .
H16A H 0.047968 0.062365 -0.126025 0.046 Uiso 1 1 calc R U . . .
H16B H 0.071350 0.125323 -0.183128 0.046 Uiso 1 1 calc R U . . .
H16C H 0.000837 0.143192 -0.123415 0.046 Uiso 1 1 calc R U . . .
C231 C 0.8682(3) 0.3183(2) 0.2443(2) 0.0227(6) Uani 1 1 d . . . . .
C232 C 0.9803(3) 0.2938(2) 0.2620(2) 0.0305(7) Uani 1 1 d . . . . .
H23A H 1.050704 0.346054 0.277576 0.046 Uiso 1 1 calc R U . . .
H23B H 0.970083 0.251218 0.210056 0.046 Uiso 1 1 calc R U . . .
H23C H 0.992868 0.268230 0.309925 0.046 Uiso 1 1 calc R U . . .
C251 C 0.8332(3) 0.5496(2) 0.1684(2) 0.0244(6) Uani 1 1 d . . . . .
C252 C 0.9341(3) 0.6142(2) 0.1578(2) 0.0316(7) Uani 1 1 d . . . . .
H25A H 1.006433 0.638214 0.212596 0.047 Uiso 1 1 calc R U . . .
H25B H 0.907766 0.661627 0.141667 0.047 Uiso 1 1 calc R U . . .
H25C H 0.953285 0.584428 0.112401 0.047 Uiso 1 1 calc R U . . .
C261 C 0.5404(3) 0.1450(2) -0.0008(2) 0.0232(6) Uani 1 1 d . . . . .
C262 C 0.5438(3) 0.0743(2) -0.0672(3) 0.0340(8) Uani 1 1 d . . . . .
H26A H 0.508006 0.017439 -0.060791 0.051 Uiso 1 1 calc R U . . .
H26B H 0.628103 0.083501 -0.058845 0.051 Uiso 1 1 calc R U . . .
H26C H 0.497508 0.075936 -0.125366 0.051 Uiso 1 1 calc R U . . .
C341 C 0.4734(3) 0.5807(2) 0.3481(2) 0.0258(6) Uani 1 1 d . . . . .
C342 C 0.4566(4) 0.6559(2) 0.4009(3) 0.0371(8) Uani 1 1 d . . . . .
H34A H 0.525270 0.709390 0.416787 0.056 Uiso 1 1 calc R U . . .
H34B H 0.452341 0.643581 0.453604 0.056 Uiso 1 1 calc R U . . .
H34C H 0.381208 0.663354 0.366715 0.056 Uiso 1 1 calc R U . . .
C351 C 0.8361(3) 0.5421(2) 0.4177(2) 0.0283(7) Uani 1 1 d . . . . .
C352 C 0.9384(4) 0.6036(3) 0.4996(3) 0.0457(10) Uani 1 1 d . . . . .
H35A H 0.910066 0.610274 0.546194 0.069 Uiso 1 1 calc R U . . .
H35B H 0.967540 0.660568 0.491027 0.069 Uiso 1 1 calc R U . . .
H35C H 1.004630 0.580369 0.515351 0.069 Uiso 1 1 calc R U . . .
O71 O 0.0531(2) 0.19534(16) 0.05956(17) 0.0331(5) Uani 1 1 d . . . . .
O72 O 0.0362(3) 0.1025(3) 0.1360(3) 0.0835(15) Uani 1 1 d . . . . .
H72 H 0.112222 0.120482 0.154560 0.125 Uiso 1 1 calc R U . . .
C71 C -0.0078(3) 0.1359(2) 0.0758(2) 0.0320(7) Uani 1 1 d . . . . .
C72 C -0.1412(4) 0.0951(4) 0.0305(3) 0.0599(13) Uani 1 1 d . . . . .
H72A H -0.178785 0.117403 0.067095 0.090 Uiso 1 1 calc R U . . .
H72B H -0.164434 0.031668 0.018488 0.090 Uiso 1 1 calc R U . . .
H72C H -0.168851 0.109248 -0.024130 0.090 Uiso 1 1 calc R U . . .
O81 O 0.7186(2) 0.12596(15) 0.17815(17) 0.0315(5) Uani 1 1 d . . . . .
O82 O 0.7161(4) 0.0804(2) 0.2917(2) 0.0587(9) Uani 1 1 d . . . . .
H82 H 0.686678 0.119580 0.300152 0.088 Uiso 1 1 calc R U . . .
C81 C 0.7379(3) 0.0782(2) 0.2220(3) 0.0352(8) Uani 1 1 d . . . . .
C82 C 0.7865(4) 0.0076(3) 0.2003(3) 0.0467(10) Uani 1 1 d . . . . .
H82A H 0.741068 -0.025370 0.138800 0.070 Uiso 1 1 calc R U . . .
H82B H 0.777665 -0.031679 0.235526 0.070 Uiso 1 1 calc R U . . .
H82C H 0.872434 0.033836 0.212393 0.070 Uiso 1 1 calc R U . . .
O1W O 0.6519(3) 0.5263(2) 0.49611(19) 0.0470(7) Uani 1 1 d D . . . .
H1W H 0.702(4) 0.509(4) 0.531(3) 0.071 Uiso 1 1 d D U . . .
H2W H 0.611(4) 0.546(4) 0.520(3) 0.071 Uiso 1 1 d D U . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0181 0.0091 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0492 0.0322 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zr Zr -0.1862 2.2449 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O136 Zr1 O145 92.65(8) . . ?
O136 Zr1 O11 85.33(8) . . ?
O145 Zr1 O11 143.00(8) . . ?
O136 Zr1 O15 87.34(8) . . ?
O145 Zr1 O15 142.92(8) . . ?
O11 Zr1 O15 74.00(8) . . ?
O136 Zr1 O12 143.01(8) . . ?
O145 Zr1 O12 84.32(8) . . ?
O11 Zr1 O12 75.83(8) . . ?
O15 Zr1 O12 116.58(8) . . ?
O136 Zr1 O14 143.11(8) . . ?
O145 Zr1 O14 86.92(8) . . ?
O11 Zr1 O14 116.02(8) . . ?
O15 Zr1 O14 71.87(8) . . ?
O12 Zr1 O14 73.70(8) . . ?
O136 Zr1 O135 68.84(7) . . ?
O145 Zr1 O135 68.98(8) . . ?
O11 Zr1 O135 141.43(8) . . ?
O15 Zr1 O135 76.58(8) . . ?
O12 Zr1 O135 140.88(8) . . ?
O14 Zr1 O135 76.71(7) . . ?
O136 Zr1 O146 71.59(7) . . ?
O145 Zr1 O146 71.78(8) . . ?
O11 Zr1 O146 72.57(8) . . ?
O15 Zr1 O146 141.55(8) . . ?
O12 Zr1 O146 72.48(7) . . ?
O14 Zr1 O146 141.39(7) . . ?
O135 Zr1 O146 121.54(7) . . ?
O136 Zr1 Zr4 83.79(6) . . ?
O145 Zr1 Zr4 33.07(6) . . ?
O11 Zr1 Zr4 110.32(6) . . ?
O15 Zr1 Zr4 169.72(5) . . ?
O12 Zr1 Zr4 73.71(6) . . ?
O14 Zr1 Zr4 112.80(6) . . ?
O135 Zr1 Zr4 95.31(5) . . ?
O146 Zr1 Zr4 38.87(5) . . ?
O136 Zr1 Zr6 32.82(6) . . ?
O145 Zr1 Zr6 84.41(6) . . ?
O11 Zr1 Zr6 74.06(5) . . ?
O15 Zr1 Zr6 112.70(5) . . ?
O12 Zr1 Zr6 110.41(6) . . ?
O14 Zr1 Zr6 169.93(6) . . ?
O135 Zr1 Zr6 95.35(5) . . ?
O146 Zr1 Zr6 38.99(5) . . ?
Zr4 Zr1 Zr6 61.207(7) . . ?
O136 Zr1 Zr5 80.85(6) . . ?
O145 Zr1 Zr5 30.49(6) . . ?
O11 Zr1 Zr5 163.62(6) . . ?
O15 Zr1 Zr5 113.84(6) . . ?
O12 Zr1 Zr5 110.63(6) . . ?
O14 Zr1 Zr5 80.36(6) . . ?
O135 Zr1 Zr5 38.50(5) . . ?
O146 Zr1 Zr5 94.61(5) . . ?
Zr4 Zr1 Zr5 59.589(7) . . ?
Zr6 Zr1 Zr5 89.566(8) . . ?
O136 Zr1 Zr2 30.14(6) . . ?
O145 Zr1 Zr2 81.33(5) . . ?
O11 Zr1 Zr2 111.12(5) . . ?
O15 Zr1 Zr2 80.32(5) . . ?
O12 Zr1 Zr2 163.10(6) . . ?
O14 Zr1 Zr2 114.19(5) . . ?
O135 Zr1 Zr2 38.71(5) . . ?
O146 Zr1 Zr2 94.47(5) . . ?
Zr4 Zr1 Zr2 89.398(8) . . ?
Zr6 Zr1 Zr2 59.396(7) . . ?
Zr5 Zr1 Zr2 58.642(7) . . ?
O235 Zr2 O136 90.69(8) . . ?
O235 Zr2 O21 85.38(8) . . ?
O136 Zr2 O21 140.76(8) . . ?
O235 Zr2 O55 145.08(8) . 2_665 ?
O136 Zr2 O55 96.14(8) . 2_665 ?
O21 Zr2 O55 109.15(8) . 2_665 ?
O235 Zr2 O22 142.43(8) . . ?
O136 Zr2 O22 81.81(8) . . ?
O21 Zr2 O22 78.03(8) . . ?
O55 Zr2 O22 72.49(8) 2_665 . ?
O235 Zr2 O25 81.64(8) . . ?
O136 Zr2 O25 144.75(8) . . ?
O21 Zr2 O25 73.17(8) . . ?
O55 Zr2 O25 73.11(8) 2_665 . ?
O22 Zr2 O25 123.86(8) . . ?
O235 Zr2 O135 70.37(8) . . ?
O136 Zr2 O135 68.57(7) . . ?
O21 Zr2 O135 143.45(8) . . ?
O55 Zr2 O135 80.39(8) 2_665 . ?
O22 Zr2 O135 137.12(8) . . ?
O25 Zr2 O135 76.49(8) . . ?
O235 Zr2 O236 69.82(8) . . ?
O136 Zr2 O236 70.24(7) . . ?
O21 Zr2 O236 71.80(7) . . ?
O55 Zr2 O236 144.36(8) 2_665 . ?
O22 Zr2 O236 73.02(8) . . ?
O25 Zr2 O236 135.98(8) . . ?
O135 Zr2 O236 120.98(7) . . ?
O235 Zr2 Zr3 31.12(6) . . ?
O136 Zr2 Zr3 83.21(6) . . ?
O21 Zr2 Zr3 73.49(6) . . ?
O55 Zr2 Zr3 175.93(6) 2_665 . ?
O22 Zr2 Zr3 111.32(6) . . ?
O25 Zr2 Zr3 105.14(6) . . ?
O135 Zr2 Zr3 95.66(5) . . ?
O236 Zr2 Zr3 39.03(5) . . ?
O235 Zr2 Zr6 81.54(6) . . ?
O136 Zr2 Zr6 32.26(6) . . ?
O21 Zr2 Zr6 108.85(6) . . ?
O55 Zr2 Zr6 120.36(6) 2_665 . ?
O22 Zr2 Zr6 72.57(6) . . ?
O25 Zr2 Zr6 162.83(6) . . ?
O135 Zr2 Zr6 94.55(5) . . ?
O236 Zr2 Zr6 38.13(5) . . ?
Zr3 Zr2 Zr6 60.646(7) . . ?
O235 Zr2 Zr5 30.90(6) . . ?
O136 Zr2 Zr5 82.25(6) . . ?
O21 Zr2 Zr5 110.66(6) . . ?
O55 Zr2 Zr5 116.39(6) 2_665 . ?
O22 Zr2 Zr5 162.54(6) . . ?
O25 Zr2 Zr5 73.58(6) . . ?
O135 Zr2 Zr5 39.77(5) . . ?
O236 Zr2 Zr5 94.86(5) . . ?
Zr3 Zr2 Zr5 59.555(7) . . ?
Zr6 Zr2 Zr5 90.109(8) . . ?
O235 Zr2 Zr1 80.82(6) . . ?
O136 Zr2 Zr1 29.78(5) . . ?
O21 Zr2 Zr1 162.44(6) . . ?
O55 Zr2 Zr1 88.33(6) 2_665 . ?
O22 Zr2 Zr1 106.78(6) . . ?
O25 Zr2 Zr1 115.09(5) . . ?
O135 Zr2 Zr1 38.80(5) . . ?
O236 Zr2 Zr1 93.15(5) . . ?
Zr3 Zr2 Zr1 89.147(8) . . ?
Zr6 Zr2 Zr1 58.483(7) . . ?
Zr5 Zr2 Zr1 60.454(7) . . ?
O235 Zr3 O346 94.36(8) . . ?
O235 Zr3 O32 84.21(8) . . ?
O346 Zr3 O32 142.22(8) . . ?
O235 Zr3 O356 73.94(8) . . ?
O346 Zr3 O356 70.05(8) . . ?
O32 Zr3 O356 143.23(8) . . ?
O235 Zr3 O31 83.63(8) . . ?
O346 Zr3 O31 143.14(8) . . ?
O32 Zr3 O31 74.39(8) . . ?
O356 Zr3 O31 74.09(8) . . ?
O235 Zr3 O236 73.14(8) . . ?
O346 Zr3 O236 69.67(8) . . ?
O32 Zr3 O236 73.88(8) . . ?
O356 Zr3 O236 124.76(8) . . ?
O31 Zr3 O236 142.14(8) . . ?
O235 Zr3 O34 150.49(8) . . ?
O346 Zr3 O34 87.44(9) . . ?
O32 Zr3 O34 76.71(8) . . ?
O356 Zr3 O34 133.34(8) . . ?
O31 Zr3 O34 111.94(9) . . ?
O236 Zr3 O34 80.00(8) . . ?
O235 Zr3 O33 152.35(8) . . ?
O346 Zr3 O33 90.19(9) . . ?
O32 Zr3 O33 108.30(9) . . ?
O356 Zr3 O33 82.11(8) . . ?
O31 Zr3 O33 76.58(9) . . ?
O236 Zr3 O33 133.46(8) . . ?
O34 Zr3 O33 56.85(8) . . ?
O235 Zr3 C35 177.04(10) . . ?
O346 Zr3 C35 88.47(10) . . ?
O32 Zr3 C35 93.03(10) . . ?
O356 Zr3 C35 107.90(9) . . ?
O31 Zr3 C35 94.62(10) . . ?
O236 Zr3 C35 107.15(10) . . ?
O34 Zr3 C35 28.65(10) . . ?
O33 Zr3 C35 28.20(10) . . ?
O235 Zr3 Zr5 31.62(6) . . ?
O346 Zr3 Zr5 85.97(6) . . ?
O32 Zr3 Zr5 109.27(6) . . ?
O356 Zr3 Zr5 42.66(5) . . ?
O31 Zr3 Zr5 73.16(6) . . ?
O236 Zr3 Zr5 98.61(5) . . ?
O34 Zr3 Zr5 173.33(6) . . ?
O33 Zr3 Zr5 122.11(6) . . ?
C35 Zr3 Zr5 149.84(8) . . ?
O235 Zr3 Zr2 31.30(6) . . ?
O346 Zr3 Zr2 85.80(6) . . ?
O32 Zr3 Zr2 73.53(6) . . ?
O356 Zr3 Zr2 99.14(6) . . ?
O31 Zr3 Zr2 108.34(6) . . ?
O236 Zr3 Zr2 42.18(5) . . ?
O34 Zr3 Zr2 120.01(6) . . ?
O33 Zr3 Zr2 175.09(7) . . ?
C35 Zr3 Zr2 148.50(8) . . ?
Zr5 Zr3 Zr2 60.479(7) . . ?
O235 Zr3 Zr4 81.26(6) . . ?
O346 Zr3 Zr4 33.15(6) . . ?
O32 Zr3 Zr4 163.72(6) . . ?
O356 Zr3 Zr4 37.05(6) . . ?
O31 Zr3 Zr4 111.02(6) . . ?
O236 Zr3 Zr4 94.79(5) . . ?
O34 Zr3 Zr4 113.43(6) . . ?
O33 Zr3 Zr4 87.97(7) . . ?
C35 Zr3 Zr4 101.61(8) . . ?
Zr5 Zr3 Zr4 60.063(7) . . ?
Zr2 Zr3 Zr4 90.209(8) . . ?
O145 Zr4 O346 96.82(8) . . ?
O145 Zr4 O356 74.72(8) . . ?
O346 Zr4 O356 70.50(8) . . ?
O145 Zr4 O146 74.24(8) . . ?
O346 Zr4 O146 70.34(8) . . ?
O356 Zr4 O146 125.71(8) . . ?
O145 Zr4 O42 84.00(8) . . ?
O346 Zr4 O42 143.19(9) . . ?
O356 Zr4 O42 143.00(8) . . ?
O146 Zr4 O42 74.60(8) . . ?
O145 Zr4 O41 81.75(8) . . ?
O346 Zr4 O41 144.45(9) . . ?
O356 Zr4 O41 74.96(8) . . ?
O146 Zr4 O41 140.66(8) . . ?
O42 Zr4 O41 72.26(9) . . ?
O145 Zr4 O43 152.49(9) . . ?
O346 Zr4 O43 91.80(9) . . ?
O356 Zr4 O43 83.75(9) . . ?
O146 Zr4 O43 133.12(8) . . ?
O42 Zr4 O43 104.33(9) . . ?
O41 Zr4 O43 76.19(9) . . ?
O145 Zr4 O44 149.64(9) . . ?
O346 Zr4 O44 85.07(8) . . ?
O356 Zr4 O44 133.16(8) . . ?
O146 Zr4 O44 78.00(8) . . ?
O42 Zr4 O44 76.96(8) . . ?
O41 Zr4 O44 113.77(8) . . ?
O43 Zr4 O44 56.99(9) . . ?
O145 Zr4 C45 175.05(9) . . ?
O346 Zr4 C45 87.58(9) . . ?
O356 Zr4 C45 109.03(10) . . ?
O146 Zr4 C45 105.30(10) . . ?
O42 Zr4 C45 91.13(9) . . ?
O41 Zr4 C45 95.99(10) . . ?
O43 Zr4 C45 28.75(10) . . ?
O44 Zr4 C45 28.25(10) . . ?
O145 Zr4 Zr1 33.23(6) . . ?
O346 Zr4 Zr1 86.17(6) . . ?
O356 Zr4 Zr1 100.57(6) . . ?
O146 Zr4 Zr1 41.18(5) . . ?
O42 Zr4 Zr1 74.50(6) . . ?
O41 Zr4 Zr1 108.46(6) . . ?
O43 Zr4 Zr1 174.27(7) . . ?
O44 Zr4 Zr1 117.45(6) . . ?
C45 Zr4 Zr1 145.64(8) . . ?
O145 Zr4 Zr5 32.54(6) . . ?
O346 Zr4 Zr5 85.59(6) . . ?
O356 Zr4 Zr5 42.24(6) . . ?
O146 Zr4 Zr5 98.94(5) . . ?
O42 Zr4 Zr5 110.94(6) . . ?
O41 Zr4 Zr5 74.22(6) . . ?
O43 Zr4 Zr5 123.26(7) . . ?
O44 Zr4 Zr5 170.66(6) . . ?
C45 Zr4 Zr5 150.88(8) . . ?
Zr1 Zr4 Zr5 61.956(7) . . ?
O145 Zr4 Zr3 83.31(6) . . ?
O346 Zr4 Zr3 33.21(6) . . ?
O356 Zr4 Zr3 37.43(5) . . ?
O146 Zr4 Zr3 95.55(5) . . ?
O42 Zr4 Zr3 165.69(6) . . ?
O41 Zr4 Zr3 112.28(6) . . ?
O43 Zr4 Zr3 89.98(6) . . ?
O44 Zr4 Zr3 111.64(6) . . ?
C45 Zr4 Zr3 101.63(7) . . ?
Zr1 Zr4 Zr3 91.233(8) . . ?
Zr5 Zr4 Zr3 59.593(7) . . ?
O235 Zr5 O145 91.57(8) . . ?
O235 Zr5 O53 85.54(8) . . ?
O145 Zr5 O53 141.79(8) . . ?
O235 Zr5 O52 145.91(8) . 2_665 ?
O145 Zr5 O52 96.84(8) . 2_665 ?
O53 Zr5 O52 106.68(9) . 2_665 ?
O235 Zr5 O54 141.82(8) . . ?
O145 Zr5 O54 81.93(8) . . ?
O53 Zr5 O54 77.33(9) . . ?
O52 Zr5 O54 72.22(8) 2_665 . ?
O235 Zr5 O51 81.63(8) . . ?
O145 Zr5 O51 145.28(8) . . ?
O53 Zr5 O51 71.93(9) . . ?
O52 Zr5 O51 72.72(8) 2_665 . ?
O54 Zr5 O51 123.31(8) . . ?
O235 Zr5 O135 70.84(8) . . ?
O145 Zr5 O135 69.29(8) . . ?
O53 Zr5 O135 142.76(8) . . ?
O52 Zr5 O135 81.39(8) 2_665 . ?
O54 Zr5 O135 138.06(8) . . ?
O51 Zr5 O135 76.35(8) . . ?
O235 Zr5 O356 70.12(7) . . ?
O145 Zr5 O356 70.31(8) . . ?
O53 Zr5 O356 72.94(8) . . ?
O52 Zr5 O356 143.59(7) 2_665 . ?
O54 Zr5 O356 72.29(8) . . ?
O51 Zr5 O356 136.07(8) . . ?
O135 Zr5 O356 121.68(8) . . ?
O235 Zr5 Zr3 31.48(6) . . ?
O145 Zr5 Zr3 83.71(6) . . ?
O53 Zr5 Zr3 74.16(6) . . ?
O52 Zr5 Zr3 177.39(6) 2_665 . ?
O54 Zr5 Zr3 110.39(6) . . ?
O51 Zr5 Zr3 105.39(5) . . ?
O135 Zr5 Zr3 96.45(5) . . ?
O356 Zr5 Zr3 38.96(5) . . ?
O235 Zr5 Zr4 81.41(6) . . ?
O145 Zr5 Zr4 32.17(6) . . ?
O53 Zr5 Zr4 110.20(6) . . ?
O52 Zr5 Zr4 121.16(6) 2_665 . ?
O54 Zr5 Zr4 73.18(6) . . ?
O51 Zr5 Zr4 162.67(6) . . ?
O135 Zr5 Zr4 94.68(5) . . ?
O356 Zr5 Zr4 38.20(5) . . ?
Zr3 Zr5 Zr4 60.344(7) . . ?
O235 Zr5 Zr2 30.94(6) . . ?
O145 Zr5 Zr2 83.28(6) . . ?
O53 Zr5 Zr2 110.38(6) . . ?
O52 Zr5 Zr2 117.53(6) 2_665 . ?
O54 Zr5 Zr2 163.23(6) . . ?
O51 Zr5 Zr2 73.45(6) . . ?
O135 Zr5 Zr2 40.20(5) . . ?
O356 Zr5 Zr2 95.27(5) . . ?
Zr3 Zr5 Zr2 59.966(7) . . ?
Zr4 Zr5 Zr2 90.076(8) . . ?
O235 Zr5 Zr1 81.25(6) . . ?
O145 Zr5 Zr1 30.29(6) . . ?
O53 Zr5 Zr1 163.70(6) . . ?
O52 Zr5 Zr1 89.58(6) 2_665 . ?
O54 Zr5 Zr1 107.64(6) . . ?
O51 Zr5 Zr1 115.16(6) . . ?
O135 Zr5 Zr1 39.00(5) . . ?
O356 Zr5 Zr1 93.49(5) . . ?
Zr3 Zr5 Zr1 89.634(8) . . ?
Zr4 Zr5 Zr1 58.455(7) . . ?
Zr2 Zr5 Zr1 60.904(7) . . ?
O136 Zr6 O346 95.70(8) . . ?
O136 Zr6 O236 74.44(8) . . ?
O346 Zr6 O236 70.01(8) . . ?
O136 Zr6 O62 82.90(8) . . ?
O346 Zr6 O62 144.92(8) . . ?
O236 Zr6 O62 75.94(8) . . ?
O136 Zr6 O146 73.61(8) . . ?
O346 Zr6 O146 69.72(8) . . ?
O236 Zr6 O146 124.73(8) . . ?
O62 Zr6 O146 140.88(8) . . ?
O136 Zr6 O61 84.53(8) . . ?
O346 Zr6 O61 141.38(8) . . ?
O236 Zr6 O61 144.74(8) . . ?
O62 Zr6 O61 73.59(8) . . ?
O146 Zr6 O61 73.41(8) . . ?
O136 Zr6 O64 151.52(8) . . ?
O346 Zr6 O64 86.37(9) . . ?
O236 Zr6 O64 131.93(8) . . ?
O62 Zr6 O64 111.23(9) . . ?
O146 Zr6 O64 80.62(8) . . ?
O61 Zr6 O64 76.59(9) . . ?
O136 Zr6 O63 151.17(8) . . ?
O346 Zr6 O63 86.71(8) . . ?
O236 Zr6 O63 79.51(8) . . ?
O62 Zr6 O63 78.95(8) . . ?
O146 Zr6 O63 133.09(8) . . ?
O61 Zr6 O63 111.15(9) . . ?
O64 Zr6 O63 57.21(8) . . ?
O136 Zr6 C65 179.20(10) . . ?
O346 Zr6 C65 83.61(9) . . ?
O236 Zr6 C65 104.93(9) . . ?
O62 Zr6 C65 97.45(9) . . ?
O146 Zr6 C65 106.47(9) . . ?
O61 Zr6 C65 96.26(9) . . ?
O64 Zr6 C65 28.90(9) . . ?
O63 Zr6 C65 28.50(9) . . ?
O136 Zr6 Zr1 32.83(5) . . ?
O346 Zr6 Zr1 85.58(6) . . ?
O236 Zr6 Zr1 100.09(5) . . ?
O62 Zr6 Zr1 108.87(6) . . ?
O146 Zr6 Zr1 41.01(5) . . ?
O61 Zr6 Zr1 73.86(6) . . ?
O64 Zr6 Zr1 119.74(6) . . ?
O63 Zr6 Zr1 171.91(6) . . ?
C65 Zr6 Zr1 147.32(7) . . ?
O136 Zr6 Zr2 32.67(6) . . ?
O346 Zr6 Zr2 85.42(6) . . ?
O236 Zr6 Zr2 41.93(5) . . ?
O62 Zr6 Zr2 74.59(6) . . ?
O146 Zr6 Zr2 98.88(5) . . ?
O61 Zr6 Zr2 111.59(6) . . ?
O64 Zr6 Zr2 171.40(7) . . ?
O63 Zr6 Zr2 119.66(6) . . ?
C65 Zr6 Zr2 146.74(7) . . ?
Zr1 Zr6 Zr2 62.121(7) . . ?
O136 Zr6 Zr4 82.02(6) . . ?
O346 Zr6 Zr4 32.92(5) . . ?
O236 Zr6 Zr4 94.93(6) . . ?
O62 Zr6 Zr4 164.04(6) . . ?
O146 Zr6 Zr4 36.94(6) . . ?
O61 Zr6 Zr4 110.04(6) . . ?
O64 Zr6 Zr4 84.64(6) . . ?
O63 Zr6 Zr4 112.68(6) . . ?
C65 Zr6 Zr4 97.57(7) . . ?
Zr1 Zr6 Zr4 59.242(7) . . ?
Zr2 Zr6 Zr4 89.840(8) . . ?
C161 O11 Zr1 134.7(2) . . ?
C141 O12 Zr1 134.5(2) . . ?
C143 O14 Zr1 145.6(2) . . ?
C151 O15 Zr1 146.25(19) . . ?
C231 O21 Zr2 134.32(19) . . ?
C261 O22 Zr2 135.1(2) . . ?
C251 O25 Zr2 134.3(2) . . ?
C351 O31 Zr3 133.4(2) . . ?
C231 O32 Zr3 132.9(2) . . ?
C35 O33 Zr3 93.0(2) . . ?
C35 O34 Zr3 92.7(2) . . ?
C341 O41 Zr4 131.9(2) . . ?
C141 O42 Zr4 132.3(2) . . ?
C45 O43 Zr4 93.0(2) . . ?
C45 O44 Zr4 91.5(2) . . ?
C251 O51 Zr5 132.7(2) . . ?
C151 O52 Zr5 138.69(19) . 2_665 ?
C351 O53 Zr5 134.5(2) . . ?
C341 O54 Zr5 135.4(2) . . ?
C143 O55 Zr2 138.6(2) . 2_665 ?
C161 O61 Zr6 132.8(2) . . ?
C261 O62 Zr6 132.6(2) . . ?
C65 O63 Zr6 92.01(19) . . ?
C65 O64 Zr6 91.96(19) . . ?
Zr5 O135 Zr2 100.03(8) . . ?
Zr5 O135 Zr1 102.50(8) . . ?
Zr2 O135 Zr1 102.49(8) . . ?
Zr6 O136 Zr1 114.34(9) . . ?
Zr6 O136 Zr2 115.07(9) . . ?
Zr1 O136 Zr2 120.08(10) . . ?
Zr4 O145 Zr1 113.70(10) . . ?
Zr4 O145 Zr5 115.29(10) . . ?
Zr1 O145 Zr5 119.22(9) . . ?
Zr4 O146 Zr6 105.86(9) . . ?
Zr4 O146 Zr1 99.95(8) . . ?
Zr6 O146 Zr1 100.00(8) . . ?
Zr3 O235 Zr5 116.90(10) . . ?
Zr3 O235 Zr2 117.58(10) . . ?
Zr5 O235 Zr2 118.16(10) . . ?
Zr6 O236 Zr3 106.03(8) . . ?
Zr6 O236 Zr2 99.94(8) . . ?
Zr3 O236 Zr2 98.79(8) . . ?
Zr4 O346 Zr3 113.64(10) . . ?
Zr4 O346 Zr6 113.79(10) . . ?
Zr3 O346 Zr6 114.01(9) . . ?
Zr4 O356 Zr3 105.51(9) . . ?
Zr4 O356 Zr5 99.56(8) . . ?
Zr3 O356 Zr5 98.37(8) . . ?
O33 C35 O34 117.5(3) . . ?
O33 C35 C36 122.3(3) . . ?
O34 C35 C36 120.2(3) . . ?
O33 C35 Zr3 58.84(18) . . ?
O34 C35 Zr3 58.65(17) . . ?
C36 C35 Zr3 178.6(3) . . ?
O44 C45 O43 118.5(3) . . ?
O44 C45 C46 121.0(3) . . ?
O43 C45 C46 120.5(3) . . ?
O44 C45 Zr4 60.27(16) . . ?
O43 C45 Zr4 58.22(16) . . ?
C46 C45 Zr4 177.3(3) . . ?
O63 C65 O64 118.0(3) . . ?
O63 C65 C66 121.4(3) . . ?
O64 C65 C66 120.5(3) . . ?
O63 C65 Zr6 59.49(16) . . ?
O64 C65 Zr6 59.14(16) . . ?
C66 C65 Zr6 170.8(3) . . ?
O42 C141 O12 124.8(3) . . ?
O42 C141 C142 118.1(3) . . ?
O12 C141 C142 117.1(3) . . ?
O14 C143 O55 121.6(3) . . ?
O14 C143 C144 121.2(3) . . ?
O55 C143 C144 117.2(3) . . ?
O15 C151 O52 122.0(3) . . ?
O15 C151 C152 121.1(3) . . ?
O52 C151 C152 117.0(3) . . ?
O61 C161 O11 124.1(3) . . ?
O61 C161 C162 119.5(3) . . ?
O11 C161 C162 116.5(3) . . ?
O21 C231 O32 124.9(3) . . ?
O21 C231 C232 117.6(3) . . ?
O32 C231 C232 117.5(3) . . ?
O25 C251 O51 125.3(3) . . ?
O25 C251 C252 117.7(3) . . ?
O51 C251 C252 117.0(3) . . ?
O22 C261 O62 125.1(3) . . ?
O22 C261 C262 117.5(3) . . ?
O62 C261 C262 117.5(3) . . ?
O54 C341 O41 125.1(3) . . ?
O54 C341 C342 117.9(3) . . ?
O41 C341 C342 117.0(3) . . ?
O31 C351 O53 124.6(3) . . ?
O31 C351 C352 117.9(3) . . ?
O53 C351 C352 117.6(3) . . ?
O71 C71 O72 124.1(3) . . ?
O71 C71 C72 124.0(4) . . ?
O72 C71 C72 111.8(3) . . ?
O81 C81 O82 124.2(3) . . ?
O81 C81 C82 122.8(4) . . ?
O82 C81 C82 113.0(3) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Zr1 O136 2.0619(19) . ?
Zr1 O145 2.067(2) . ?
Zr1 O11 2.192(2) . ?
Zr1 O15 2.203(2) . ?
Zr1 O12 2.209(2) . ?
Zr1 O14 2.217(2) . ?
Zr1 O135 2.306(2) . ?
Zr1 O146 2.309(2) . ?
Zr1 Zr4 3.4537(4) . ?
Zr1 Zr6 3.4647(3) . ?
Zr1 Zr5 3.5767(4) . ?
Zr1 Zr2 3.5925(3) . ?
Zr2 O235 2.047(2) . ?
Zr2 O136 2.085(2) . ?
Zr2 O21 2.192(2) . ?
Zr2 O55 2.192(2) 2_665 ?
Zr2 O22 2.214(2) . ?
Zr2 O25 2.220(2) . ?
Zr2 O135 2.3014(19) . ?
Zr2 O236 2.373(2) . ?
Zr2 Zr3 3.4929(3) . ?
Zr2 Zr6 3.4981(3) . ?
Zr2 Zr5 3.5109(3) . ?
Zr3 O235 2.037(2) . ?
Zr3 O346 2.096(2) . ?
Zr3 O32 2.211(2) . ?
Zr3 O356 2.211(2) . ?
Zr3 O31 2.222(2) . ?
Zr3 O236 2.226(2) . ?
Zr3 O34 2.278(2) . ?
Zr3 O33 2.283(2) . ?
Zr3 C35 2.664(3) . ?
Zr3 Zr5 3.4784(3) . ?
Zr3 Zr4 3.5049(3) . ?
Zr3 Zr6 3.5295(4) . ?
Zr4 O145 2.058(2) . ?
Zr4 O346 2.092(2) . ?
Zr4 O356 2.192(2) . ?
Zr4 O146 2.201(2) . ?
Zr4 O42 2.229(2) . ?
Zr4 O41 2.247(2) . ?
Zr4 O43 2.258(2) . ?
Zr4 O44 2.304(2) . ?
Zr4 C45 2.653(3) . ?
Zr4 Zr5 3.4950(3) . ?
Zr4 Zr6 3.5221(4) . ?
Zr5 O235 2.045(2) . ?
Zr5 O145 2.079(2) . ?
Zr5 O53 2.170(2) . ?
Zr5 O52 2.185(2) 2_665 ?
Zr5 O54 2.217(2) . ?
Zr5 O51 2.252(2) . ?
Zr5 O135 2.281(2) . ?
Zr5 O356 2.383(2) . ?
Zr6 O136 2.061(2) . ?
Zr6 O346 2.113(2) . ?
Zr6 O236 2.193(2) . ?
Zr6 O62 2.202(2) . ?
Zr6 O146 2.214(2) . ?
Zr6 O61 2.236(2) . ?
Zr6 O64 2.265(2) . ?
Zr6 O63 2.274(2) . ?
Zr6 C65 2.637(3) . ?
O11 C161 1.273(4) . ?
O12 C141 1.266(4) . ?
O14 C143 1.264(4) . ?
O15 C151 1.260(4) . ?
O21 C231 1.265(4) . ?
O22 C261 1.267(4) . ?
O25 C251 1.257(4) . ?
O31 C351 1.266(4) . ?
O32 C231 1.267(4) . ?
O33 C35 1.261(4) . ?
O34 C35 1.279(4) . ?
O41 C341 1.274(4) . ?
O42 C141 1.261(4) . ?
O43 C45 1.278(4) . ?
O44 C45 1.256(4) . ?
O51 C251 1.268(4) . ?
O52 C151 1.265(4) . ?
O53 C351 1.269(4) . ?
O54 C341 1.254(4) . ?
O55 C143 1.269(4) . ?
O61 C161 1.265(4) . ?
O62 C261 1.269(4) . ?
O63 C65 1.259(4) . ?
O64 C65 1.275(4) . ?
C35 C36 1.486(5) . ?
C45 C46 1.497(5) . ?
C65 C66 1.493(5) . ?
C141 C142 1.504(4) . ?
C143 C144 1.491(4) . ?
C151 C152 1.503(4) . ?
C161 C162 1.496(5) . ?
C231 C232 1.507(4) . ?
C251 C252 1.518(4) . ?
C261 C262 1.502(4) . ?
C341 C342 1.511(4) . ?
C351 C352 1.496(5) . ?
O71 C71 1.222(4) . ?
O72 C71 1.290(5) . ?
C71 C72 1.479(5) . ?
O81 C81 1.206(4) . ?
O82 C81 1.314(5) . ?
C81 C82 1.498(5) . ?
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
_geom_hbond_publ_flag
O135 H135 O14 1.05 2.04 2.802(3) 127.0 2_665 yes
O135 H135 O15 1.05 1.87 2.821(3) 149.4 2_665 yes
O146 H146 O71 1.03 1.70 2.728(3) 177.7 . yes
O236 H236 O81 0.92 1.88 2.750(3) 156.2 . yes
O356 H356 O1W 0.95 1.70 2.616(4) 161.7 . yes
C144 H14F O145 0.98 2.52 3.359(4) 143.3 . yes
C152 H15A O136 0.98 2.57 3.396(4) 142.5 . yes
C162 H16A O72 0.98 2.62 3.590(5) 170.7 2 yes
C252 H25B O11 0.98 2.61 3.538(4) 158.3 2_665 yes
C262 H26A O62 0.98 2.62 3.485(4) 147.0 2_655 yes
C352 H35C O31 0.98 2.57 3.526(5) 166.6 2_766 yes
O72 H72 O44 0.84 2.43 2.971(5) 122.6 . yes
O72 H72 O64 0.84 2.01 2.785(4) 152.9 . yes
C72 H72A O81 0.98 2.64 3.579(6) 160.0 1_455 yes
O82 H82 O34 0.84 1.84 2.654(4) 162.6 . yes
O1W H2W O43 0.845(10) 2.06(3) 2.801(4) 146(5) 2_666 yes
